Materials Science and Engineering A284 (2000) 184 194 www.elsevier.com/locate/msea
Hot working of commercial Ti6Al4V with an equiaxed a b microstructure: materials modeling considerationsT. Seshacharyulu, S.C. Medeiros, W.G. Frazier *, Y.V.R.K. PrasadMaterials Process Design Branch (AFRL /MLMR), Materials and Manufacturing Directorate, Air Force Research Laboratory, Wright -Patterson Air Force Base, OH 45433 -7746, USA Received 14 October 1999; received in revised form 11 January 2000
Abstract The hot deformation behavior of Ti6Al4V with an equiaxed a b preform microstructure is modeled in the temperature range 7501100C and strain rate range 0.0003100 s 1, for obtaining processing windows and achieving microstructural control during hot working. For this purpose, a processing map has been developed on the basis of ow stress data as a function of temperature, strain rate and strain. The map exhibited two domains: (i) the domain in the a b phase eld is identied to represent ne-grained superplasticity and the peak efciency of power dissipation occurred at about 825C/0.0003 s 1. At this temperature, the hot ductility exhibited a sharp peak indicating that the superplasticity process is very sensitive to temperature. The a grain size increased exponentially with increase in temperature in this domain and the variation is similar to the increase in the b volume fraction in this alloy. At the temperature of peak ductility, the volume fraction of b is about 20%, suggesting that sliding of a a interfaces is primarily responsible for superplasticity while the b phase present at the grain boundary triple junctions restricts grain growth. The apparent activation energy estimated in the a b superplasticity domain is about 330 kJ mol 1, which is much higher than that for self diffusion in a-titanium. (ii) In the b phase eld, the alloy exhibits dynamic recrystallization and the variation of grain size with temperature and strain rate could be correlated with the Zener Hollomon parameter. The apparent activation energy in this domain is estimated to be 210 kJ mol 1, which is close to that for self diffusion in b. At temperatures around the transus, a ductility peak with unusually high ductility has been observed, which has been attributed to the occurrence of transient superplasticity of b in view of its ne grain size. The material exhibited ow instabilities at strain rates higher than about 1 s 1 and these are manifested as adiabatic shear bands in the a b regime. Published by Elsevier Science S.A.Keywords: Hot deformation behavior; Ti6Al4V; Equiaxed a b microstructure
1. Introduction Ti6Al4V (Ti 6 4) alloy is a two-phase alloy, which has low density and attractive mechanical and corrosion resistant properties that make it an ideal choice for many aerospace applications . It is commercially available in two grades low oxygen (ELI) grade and high oxygen (commercial) grade. It is the high oxygen grade that is widely used in gas turbine engine parts, chemical reactors and bioengineering applications. The alloy may be heat treated  to obtain a variety of microstructures ranging from b-transformed
* Corresponding author. Tel.: + 1-937-90444325; fax: + 1-9376567995. E -mail address: firstname.lastname@example.org (W.G. Frazier) 0921-5093/00/$ - see front matter Published by Elsevier Science S.A. PII: S 0 9 2 1 - 5 0 9 3 ( 0 0 ) 0 0 7 4 1 - 3
(martensitic/lamellar) to equiaxed a b. Bulk mechanical processing of this material to manufacture semiproducts includes ingot breakdown at temperatures above the b transus and conversion of transformed b lamellar structure into equiaxed a b by subtransus deformation . The nishing operations for component manufacture are generally conducted  on the equiaxed structure in the a b phase eld during which only minor changes in the microstructure take place. One of the very common industrial processes used for this purpose is superplastic forming, which requires very ne grain sizes and slow speeds of deformation [7,8]. The characteristics of superplastic deformation in Ti64 have been studied extensively in the literature . Although superplastic elongations have been recorded by several investigators, there are reports of cavity formation at higher strains and lower tempera-
T. Seshacharyulu et al. / Materials Science and Engineering A284 (2000) 184194
tures ( B 850C) [12,15]. The constitutive behavior of commercial grade Ti 6 4 during hot deformation in the a b range has been characterized by Sheppard and Norley in torsion  and Seetharaman et al. in compression  and microstructural mechanisms have been identied to be dynamic recrystallization (DRX) and spheroidization respectively. The objective of this study is to model the microstructural mechanisms of hot deformation of commercial Ti64 with an equiaxed a b microstructure over a wide range of temperature and strain rate such that windows for industrial processing may be identied for optimizing workability and controlling microstructure. To reach this objective, the characteristics of the alloy have been studied in the temperature ranges covering not only a b and b phase elds but also the transus. Likewise, a wide strain rate range that encompasses the speeds of commonly used machines in the industry like hydraulic presses (slow), mechanical/friction screw presses and hammers (medium), continuous rolling and ring rolling (fast) mills, is investigated. Several approaches of materials modeling are in vogue and these include analysis of shapes of stress strain curves , kinetic analysis , and processing maps  and these have been reviewed recently . Although all the approaches have been followed in this paper, the emphasis has been on processing maps since this approach has been found to be consistent in predicting the behavior of a wide range of materials . In brief, the processing maps consist of a superimposition of power dissipation maps and instability maps developed in a frame of temperature and strain rate. The power dissipation maps represent the pattern in which the power is dissipated by the material through microstructural changes. The rate of this change is given by a dimensionless parameter called the efciency of power dissipation:
where m is strain rate sensitivity of ow stress. Over this frame is superimposed a continuum instability criterion for identifying the regimes of ow instabilities, developed on the basis of extremum principles of irreversible thermodynamics as applied to large plastic ow  and given by: x (m; ) = ( ln(m /m + 1) +mB0 ( ln m; (2)
where x (m; ) is a dimensionless instability parameter and m; is the applied strain rate. Flow instabilities are predicted to occur when x (m; ) becomes negative. The processing maps exhibit domains in which specic microstructural mechanisms operate as well as regimes where there will be ow instabilities like adiabatic shear bands or ow localization.
2. Materials and procedures
2.1. MaterialCommercial grade Ti64 having the following composition (wt.%) was used in this study: 6.28 Al, 3.97 V, 0.18 O, 0.052 Fe, 0.0062 N, 0.008 C, 0.0049 H, and balance Ti. The b transus for this material is about 1010C. As received bar stocks of 20 mm diameter in the mill annealed condition were used for testing and the starting microstructure is shown in Fig. 1. It consisted of equiaxed a grains of about 8 mm average diameter with a small amount of intergranular b.
2.2. Hot compression testingCompression specimens of 15 mm height and 10 mm diameter were machined for testing in the a + b range, while larger specimens of 22.5 mm height and 15 mm diameter were used to obtain an accurate measurement of the ow stress in the b range. Concentric grooves of 0.5 mm depth were made on the top and bottom faces of the specimens to trap lubricant and assist in reducing friction. A 1-mm 45 chamfer was provided on the specimen edges to avoid fold-over of the material during the initial stages of compression. A small hole of 0.8 mm diameter and 5 mm depth was drilled at mid height of the specimen for inserting a thermocouple which is used to measure the actual temperature of the specimen as well as adiabatic temperature rise, if any, during testing. Isothermal hot compression tests were conducted using a servohydraulic testing machine. A resistance heating split furnace with SiC elements was used to surround the platens and specimen. The specimens were coated with a borosilicate glass paste for lubrication and environmental protection.
Fig. 1. Starting microstructure of Ti6Al4V used in this study.
T. Seshacharyulu et al. / Materials Science and Engineering A284 (2000) 184194
cubic spline t between log | and log m; was used to obtain the strain rate sensitivity (m ) as a function of strain rate. This was repeated at different temperatures. The efciency of power dissipation (p ) through microstructural changes was then calculated as a function of temperature and strain rate using Eq. (1) and plotted as an iso-efciency contour map. The data were also used to evaluate the ow instability parameter x (m; ) using Eq. (2) as a function of temperature and strain rate to develop an instability map.
2.4. Hot tensile testingHot tensile tests were conducted in the temperature range 8001100C at a nominal strain rate of 0.01 s 1 (constant actuator speed of 0.25 mm s 1). Cylindrical specimens of 25 mm gauge length and 4 mm diameter were used for this purpose. The specimens were pulled to fracture and total elongation as a function of temperature was recorded. 3. Results and discussion
3.1. Stress strain beha6iorThe shapes of stressstrain curves indicate some features that help in identifying the mechanisms of hot deformation, although not in a conclusive fashion. Commerci